Date post: | 01-Jun-2020 |

Category: | ## Documents |

View: | 0 times |

Download: | 0 times |

Share this document with a friend

Transcript:

Quantum Dynamics of Photoinduced Electron-Transfer Reactions in Dye-SemiconductorSystems: First-Principles Description and Application to Coumarin 343-TiO2

Ivan Kondov,†,| Martin Č ı́žek,‡ Claudia Benesch,† Haobin Wang,*,§ and Michael Thoss*,†

Department of Chemistry, Technical UniVersity of Munich, Lichtenbergstrasse 4, D-85747 Garching, Germany,Institute of Theoretical Physics, Faculty of Mathematics and Physics, Charles UniVersity, Prague,Czech Republic, and Department of Chemistry and Biochemistry, MSC 3C, New Mexico State UniVersity,Las Cruces, New Mexico 88003

ReceiVed: March 20, 2007; In Final Form: May 25, 2007

A method to describe the quantum dynamics of photoinduced heterogeneous electron-transfer processes atdye-semiconductor interfaces is proposed. The method is based on a model Hamiltonian, the parameters ofwhich are determined by first-principles electronic structure calculations and a partitioning scheme to definelocalized donor and acceptor states as well as donor-acceptor coupling matrix elements. On the basis of thismodeling procedure, accurate quantum dynamical simulations are performed employing the multilayermulticonfiguration time-dependent Hartree method. As a representative example, applications to coumarin343 adsorbed on titanium oxide nanoparticles are presented. The results of the simulations show that theultrafast electron-injection process in this system is accompanied by electronic coherence effects, which arepartially quenched due to electronic-nuclear coupling.

I. Introduction

Photoinduced electron-transfer (ET) reactions at dye-semiconductor interfaces represent an interesting class of ETprocesses. In particular, the process of electron injection froman electronically excited state of a dye molecule into asemiconductor substrate has been investigated in great detailexperimentally in recent years.1-17 This process represents akey step for photonic energy conversion in nanocrystalline solarcells.2,6,9,18,19Employing femtosecond spectroscopy techniques,it has been demonstrated that electron-injection processes atdye-semiconductor interfaces often take place on an ultrafast(sub-picosecond) time scale.3,8,9,11,13,14,20For example, electron-injection times as fast as 6 fs have been reported for alizarinadsorbed on TiO2 nanoparticles14 in time-resolved experiments,and even faster ET times have been found for biisonicotinicacid on a TiO2 surface employing resonant photoemissionspectroscopy.11 Other interesting aspects of these ultrafastinterfacial ET reactions are the nonequilibrium character andthe influence of electronic-nuclear coupling. For example,studies of dye-semiconductor systems with electron-injectiontime scales on the order of a few tens to a few hundredfemtoseconds indicate that the coupling of the electronicdynamics to the nuclear (i.e., vibrational) motion of thechromophore may have a significant impact on the injectionprocess.8,20 As a result of this correlated electronic-nucleardynamics, the electron injection in these systems is often not asimple exponential decay process and thus cannot be character-ized by a single rate constant.

The theoretical study of such interfacial ET processes requiresa quantum mechanical description of the electron-injection

dynamics including the coupling to the nuclear degrees offreedom. Since it is currently not feasible to carry out a fullquantum dynamical simulation of the interfacial ET dynamicsthat takes into account the coupling to the nuclear degrees offreedom and employs an adequate electronic structure theory,different approximate strategies have been applied. One pos-sibility is to use a first-principles electronic structure methodto describe the dye-semiconductor system but employ anapproximate treatment of the nuclear motion. An example isab initio molecular dynamics, where the dynamics of the nucleardegrees of freedom are described classically.21-26 Anotherstrategy, which is particularly useful if an accurate, fullyquantum dynamical treatment is required, is to use a physicallymotivated model. A commonly used model to study heteroge-neous ET processes at interfaces is the Anderson-Newnsmodel.27 Along this line, several workers have studied theelectron-injection dynamics based on models of reduced di-mensionality, taking into account typically a single reactionmode.17,28-36 Dissipative effects, such as vibrational relaxationof the reaction mode, have been considered (for weak coupling)within Redfield theory.31 In a recent model study, we haveinvestigated in detail the influence of multidimensional coherentand dissipative vibrational motion on the electron-injectiondynamics,37 employing the self-consistent hybrid approach38,39

in combination with the multilayer multiconfiguration time-dependent Hartree method.40 These methods allow an accuratequantum dynamical description of the ET process beyond thelimitations of perturbation theory.

To apply such models to experimentally studied systems,various model parameters such as the energies and couplingsof the relevant electronic states, the important vibrational modesof the chromophore, and the electronic-vibrational couplingsneed to be determined. If only a single (or a few) reactionmode(s) is considered and a simple model for the donor-acceptor coupling (e.g., the wide-band approximation) is used,then it is possible to determine the parameters empirically based

* Authors to whom correspondence should be addressed. E-mail:[email protected] (H.W.) and [email protected] (M.T.).

† Technical University of Munich.‡ Charles University.§ New Mexico State University.| Present address: Institute for Scientific Computing, Forschungszentrum

Karlsruhe, P.O. Box 3640, 76021 Karlsruhe, Germany.

11970 J. Phys. Chem. C2007,111,11970-11981

10.1021/jp072217m CCC: $37.00 © 2007 American Chemical SocietyPublished on Web 07/21/2007

on experimental spectra.17 To simulate interfacial ET dynamicsin systems with multidimensional nuclear dynamics, we haverecently employed a semiempirical strategy, where the vibra-tional modes and electronic-vibrational couplings were deter-mined by electronic structure calculations,41,42 while for thedonor-acceptor coupling and the description of the semicon-ductor substrate an empirically parametrized tight-binding modelwas utilized.43,41As a step toward a fully first-principles-baseddescription of quantum dynamics in dye-semiconductor sys-tems, we propose here a method to determine the electronicenergies and donor-acceptor coupling matrix elements fromelectronic structure calculations.

The determination of donor-acceptor couplings in ETreactions requires, in principle, the definition of charge-localizeddiabatic states. To this end, several different approaches havebeen proposed, including the Mulliken-Hush method44,45 andits generalization46,47as well as the fragment charge differenceapproach.48 Besides these methods, which are specific to theET problem, there exist a variety of general diabatizationschemes.49 The introduction of charge-localized diabatic statesfor dye-semiconductor systems involves the additional com-plication that a (quasi-)continuum of acceptor states (corre-sponding to the (quasi-)conduction band of the semiconductornanoparticle or surface) has to be treated. Thus, the probleminvolves the treatment of a single (or a small set of) discretedonor state(s), which is (are) embedded in a (quasi-)continuumof acceptor states. This problem is closely related to thetreatment of resonances in scattering theory, e.g., electronicresonance states in low-energy electron-molecule scattering.In this context, the projection-operator approach50 has beenproven to be a very useful concept to introduce localized diabaticstates.51-53 For the present problem, we employ a method thatis similar to the projection-operator approach. The method isbased on a partitioning of the overall Hilbert space into a donorand acceptor part and a subsequent separate diagonalization ofthe two blocks of the Hamiltonian to define the donor andacceptor states. As a first step, in the present paper we workwithin the mean-field single-electron picture and use atomicorbitals to introduce the partitioning. A treatment within corre-lated many-electron states will be the subject of future work.

II. Theory

In this section, the theoretical methodology used to describephotoinduced ET reactions in dye-semiconductor systems isoutlined. The major focus is thereby on the method to determineelectronic energies and donor-acceptor coupling matrix ele-ments. To keep the paper self-contained, we also discuss brieflythe method used to describe the nuclear degrees of freedom aswell as the dynamical approach employed in the simulation.

A. Electron-Transfer Hamiltonian. To study ET dynamicsin dye-semiconductor systems, we use an ab initio (first-principles)-based model for heterogeneous ET reactions. Withinthis model the Hamiltonian is represented in a basis of thefollowing diabatic (charge-localized) electronic states that arerelevant for the photoreaction: the electronic ground state ofthe overall system|ψg〉, the donor state of the ET process|ψd〉(which, in the limit of vanishing coupling between chromophoreand semiconductor substrate, corresponds to the product of anelectronically excited state of the chromophore and an emptyconduction band of the semiconductor), and the (quasi-)-continuum of acceptor states of the ET reaction|ψk〉 (corre-sponding in the zero coupling limit to the product of the cationicstate of the chromophore and a conduction band state of thesemiconductor substrate). Thus, the Hamiltonian reads

with the kinetic energy of the nuclei (we use mass-scaledcoordinates and atomic units throughout the paper)

the potential energy in the electronic ground state,Vg(Q), andthe diabatic (donor-acceptor) potential matrixVij(Q), whichdepend on the nuclear coordinatesQ. The diagonal elementsof the diabatic potential matrix,Vdd andVkk, describe the energiesof the electronic donor and acceptor states, respectively, whilethe nondiagonal elements,Vdk, characterize the donor-acceptorET coupling.

The potential energy in the electronic ground state,Vg, can(at least in principle) rather straightforwardly be determined withelectronic structure calculations. As discussed in the introduc-tion, the characterization of the diabatic (donor-acceptor)potential matrix Vij, however, requires the introduction ofsuitable diabatic donor and acceptor states,|ψd〉 and |ψk〉.

B. Determination of Electronic Energies and Donor-Acceptor Coupling Matrix Elements. In our previous workon heterogeneous ET,37,41we have used a semiempirical method,motivated by the Newns model of chemisorption,27 with aparametrization based on a tight-binding model,43 to characterizethe diabatic states|ψd〉 and |ψk〉 and thus to determine theelectronic energies and donor-acceptor coupling matrix ele-ments Vdk. In the following, we will refer to it as thesemiempirical Newns model.

As a first step toward a first-principles description of quantumdynamics in dye-semiconductor systems, we use here anapproach based on electronic structure calculations. This ap-proach is motivated by the projection-operator approach ofresonant electron-molecule scattering.53 Specifically, we em-ploy a partitioning scheme based on density functional theory(DFT) calculations for a complex of the dye molecule with afinite TiO2 cluster. The scheme for defining the diabatic states|ψd〉 and |ψk〉 in the Hamiltonian (eq 2.1) is based on threesteps: (i) a partitioning of the Hilbert space in a donor andacceptor group using a localized basis, (ii) a partitioning of theHamiltonian according to the donor-acceptor separation, and(iii) a separate diagonalization of the donor and acceptor blocksof the partitioned Hamiltonian.54 In the present paper, we workwithin the mean-field single-electron picture. Thus we identifythe effective Hamiltonian with the Fock (or Kohn-Sham) matrixand use the orbitals and orbital energies in the partitioningmethod.

Various types of localized basis functions can be used toseparate the donor and acceptor space. Here, we employ theatomic orbitals|æj〉 used in the electronic structure calculationfor the overall system. The atomic orbitals are based on Gaussianfunctions, which are well localized in space. The set of atomicorbitals of the overall system,|æj〉, is divided into two groupssthe donor group (|æjd〉), which comprises the orbitals centeredat the atoms of the dye molecule, and the acceptor group(|æja〉), which includes the orbitals centered at the TiO2 cluster.

Since it is advantageous to work with orthogonal orbitals,55,56

the set of atomic orbitals of the overall system is orthogonalizedaccording to Lo¨wdin57,58

Hs ) T + |ψg〉Vg〈ψg| + |ψd〉Vdd〈ψd| +∑k

|ψk〉Vkk〈ψk| +

∑k

(|ψd〉Vdk〈ψk| + |ψk〉Vkd〈ψd|) (2.1)

T )1

2∑

l

Pl2 (2.2)

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711971

whereSdenotes the atomic orbital overlap matrix with elementsSkl ) 〈æk|æl〉. The new basis functions obtained,|æ̃n〉, exhibit aminimal deviation from the original ones in a least-square sense,and hence, their localization is preserved. In particular, theclassification as donor (|æ̃nd〉) or acceptor (|æ̃na〉) orbitals is stillvalid. In contrast to other orthogonalization procedures, suchas the Gram-Schmidt method, the symmetric orthogonalizationaccording to Lo¨wdin has also the advantage that it is “leastbiased”.

The new set of orthogonal basis functions is then used topartition the Fock (or Kohn-Sham) matrix from the convergedSCF (DFT) calculation into the two (donor and acceptor)subspaces. The Fock matrix in the orthogonal basis is given by

whereF denotes the Fock matrix in the original atomic orbitalbasis. The Fock matrix can be arranged in the following donor-acceptor block structure

where the matrix elements are given by

Here,f is the Fock operator,|øi〉 denote the molecular orbitalsresulting from the SCF calculation, i.e.,f |øi〉 ) �i|øi〉, and theGreek indicesR and â denote either the donor (“d”) or theacceptor (“a”) subspace.

Separate diagonalization of the two (donor and acceptor)blocks of the Fock matrixF̃RR via

and transformation of the off-diagonal parts to the correspondingeigenstates in the two blocks

result in the following prediagonalized block structure

The corresponding donor and acceptor molecular orbitals,|æj nR〉, are given as the eigenvectors ofF̃RR and are related to theorthogonalized atomic orbitals|æ̃jR〉 and the original atomicorbitals |æl〉 via

The diagonal blocks of the Fock matrix (eq 2.9) with indicesd anda contain the energies of the localized chromophore statesand those of the cluster, respectively. The off-diagonal blockscontain the electronic coupling elements between chromophoreand cluster sites. Identifying the donor state|ψd〉 with one ofthe states|æj nd〉 (based, e.g., on the orbital energy or thetransition dipole moment to the ground state) and the acceptorstates|ψk〉 with the states|æj ka〉, the electronic energies and thedonor acceptor matrix elements are given byVdd ) �d,n, Vkk )�a,k, andVdk ) Fhda,nk, respectively. It is obvious that this methodcan also be used in cases where several donor states are involvedin the ET reaction.

The partitioning method discussed above is not limited todye-semiconductor systems with a finite semiconductor clusterbut can, in principle, also be applied to a dye molecule adsorbedon an extended surface. One possibility is to employ a slabmodel and electronic structure calculations with periodic bound-ary conditions. Alternatively, the effect of an infinite semicon-ductor substrate can also be described using surface Green’sfunction techniques.59 Within this method, the effect of theinfinite substrate enters via the self-energy. In the applicationconsidered below, we have used a simpler approximate versionof this method to mimic the effect of an extended surface.Thereby a constant imaginary part is added to the atomic orbitalenergies (in the orthogonal basis|æ̃ja〉) at the outer atoms of theTiO2 cluster. The details of this method are described in theAppendix.

C. Characterization of Nuclear Degrees of Freedom.Tocharacterize the nuclear degrees of freedom, the partitioningprocedure outlined above has to be performed for each nucleargeometry, thus resulting in diabatic potential energy surfacesVii(Q) and coordinate-dependent donor-acceptor couplingmatrix elementsVdk(Q). If many nuclear degrees of freedomare important, as in the system considered below, such a globalcharacterization of the potential energy surfaces is not feasible.A more practical, local procedure is to employ the normal modes(Q) of the electronic ground state and expand the diabaticpotential matrix elementsVij(Q) around the equilibrium geom-etry of the ground state of the overall system. This approach isappropriate for photoinduced ultrafast dynamics in systemswithout large amplitude motion. It has been applied recentlyfor the related problem of molecular conduction through ametal-molecule-metal junction.60

For the present purpose of testing the partitioning procedure,we adopt the strategy used in our previous work, where thevibrational parameters and electronic-vibrational couplingparameters are determined based on electronic structure calcula-tions for the isolated chromophore, thereby neglecting thecoupling to the semiconductor substrate and to the phonons ofthe semiconductor. The extension of the method to include thisinteraction will be presented in a future publication.

The approach has been described in detail elsewhere.41

Briefly, we perform a vibrational analysis of the isolatedchromophore in the electronic ground state and employ theharmonic approximation for the corresponding potential energysurface

Here,Ql denotes thelth normal mode (with frequencyΩl), and�g is the ground-state equilibrium energy. The latter is obtainedfrom an electronic structure calculation for the overall (dye-semiconductor) system. We assume the donor-acceptor cou-

|æ̃n〉 ) ∑j

(S-1/2)jn|æj〉 (2.3)

F̃ ) S-1/2FS-1/2 (2.4)

F̃ ) (F̃dd F̃daF̃ad F̃aa) (2.5)F̃Râ,nm ) 〈æ̃n

R|f |æ̃mâ 〉) ∑

i

〈æ̃nR|øi〉�i〈øi|æ̃mâ 〉 (2.6)

FhRR ) DR†F̃RRDR (2.7)

FhRâ ) DR†F̃RâDâ (2.8)

Fh ) (Fhdd FhdaFhad Fhaa) ) (�d,1 0 ...0 �d,2 ... Fhdal l �a,1 0 ...Fhad 0 �a,2 ...l l

) (2.9)|æj nR〉 ) ∑

j

(DR)jn|æ̃jR〉

) ∑j,l

(DR)jn(S-1/2)lj|æl〉 (2.10)

Vg(Q) ) �g +1

2∑

l

Ωl2Ql

2 (2.11)

11972 J. Phys. Chem. C, Vol. 111, No. 32, 2007 Kondov et al.

pling matrix elementsVdk to be approximately independent ofthe nuclear geometry61 and expand the diabatic potential energysurfaces around the equilibrium geometry of the electronicground state,Q0

In the simplest approximation, only the linear term of theexpansion is taken into account. The frequencies are ap-proximated by their ground-state values, and Dushinsky rota-tion62 of the normal modes is neglected. In this way we obtain

This approximation has been used successfully to describeFranck-Condon and resonance Raman spectra.63 It is also usedin the linear vibronic coupling model of conical intersections64

and in the Marcus theory of ET.65

Within the description of the nuclear degrees of freedomemployed here, the parameters of the diabatic potential energysurfaces of the donor and acceptor states are obtained from thepotential energy functions of the excited state of the neutralchromophore and the ground state of the cation of the chro-mophore, respectively. Accordingly, we have

where�d and �k denote the energy of the donor and acceptorstates (at the equilibrium geometry of the ground state),respectively, which are obtained from an electronic structurecalculation of the overall system. The electronic-vibrationalcoupling constants,κl

d andκla, are obtained from the gradients

of the excited state of the neutral chromophore (correspondingto the donor state) and the ground state of the cation of thechromophore (corresponding to the acceptor state) at theequilibrium geometry of the ground state of the neutralchromophore. The details of the electronic structure calculationsas well as the specific parameters for the system consideredbelow (coumarin 343 at titanium oxide) are described else-where.41,42

In most experiments on electron injection in dye-semicon-ductor systems, a colloidal solution of dye-sensitized nanopar-ticles was employed.3,5,6,13To account for the influence of thesurrounding solvent on the ET dynamics in our simulations,we employ a standard (outer-sphere) linear response model66-68

where the Hamiltonian of the dye-semiconductor system iscoupled linearly to a bath of harmonic oscillators. Thus theHamiltonian of the overall system reads

with Hs given by eq 2.1 and

The parameters of the solvent part of the Hamiltonian arecharacterized by the spectral densities

in the donor and acceptor states, respectively. The spectraldensities describe the response of the solvent polarization tothe change of the charge distribution of the solute associatedwith electronic transitions from the ground electronic state tothe excited state of the chromophore and to the cation,respectively. In principle, the spectral densities can be differentfor the two electronic transitions. Here we use for simplicity amodeling where the response of the solvent for both transitionsis described by a coupling to the same bath that differs only inthe overall coupling strength, i.e.,cj

a ) Rcjd. (Accordingly, in

the following the superscript for the coupling constants will beomitted, i.e.,cj ≡ cjd.) It is emphasized that this approximationis only invoked for the solvent bath modes but not for theintramolecular modes. This description is in accordance withsimple dielectric continuum theories of relaxation in polarsolvents.41,68-70 As a result of this assumption, we have

The solvent reorganization energies associated with thetransitions from the electronic ground to the excited state andto the cation of the chromophore are given by

The solvent reorganization energy for the ET process, whichcorresponds to a transition from the electronically excited stateto the cation of the chromophore, however, is given by

As has been discussed in detail in ref 41, the spectral densitiesof the solvent model are chosen to be of bimodal form

with a Gaussian part accounting for the ultrafast inertialdynamics of the solvent polarization and a Debye part describingthe slower diffusive decay. The corresponding parameters,ωG) 144 cm-1, ωD ) 25 cm-1, λD

d ) λGd ) 700 cm-1, andR )

-0.1, have been chosen in accordance with experimental results

Vjj(Q) ) Vjj(Q0) + ∑l

κ ljQl + ∑

l,k

γ lkj QlQk (2.12)

Vjj(Q) ) Vjj(Q0) + ∑l

κ ljQl +

1

2∑

l

Ωl2Ql

2 (2.13)

Vdd(Q) ) �d + ∑l

κldQl +

1

2∑

l

Ωl2Ql

2 (2.14a)

Vkk(Q) ) �k + ∑l

κlaQl +

1

2∑

l

Ωl2Ql

2 (2.14b)

H ) Hs + Hb + Hsb (2.15)

Hb )1

2∑

j

(pj2 + ωj

2xj2) (2.16a)

Hsb ) |ψd〉 ∑j

cjdxj 〈ψd| + ∑

k

|ψk〉 ∑j

cjaxj 〈ψk| (2.16b)

Jd(ω) )π

2∑

j

(cjd)2

ωjδ(ω - ωj) (2.17a)

Ja(ω) )π

2∑

j

(cja)2

ωjδ(ω - ωj) (2.17b)

Jba(ω) ) R2Jb

d(ω) ) R2π

2∑

j

cj2

ωjδ(ω - ωj) (2.18)

λd ) ∑j

(cjd)2

2ωj2≡ ∑

j

cj2

2ωj2

(2.19a)

λa ) ∑j

(cja)2

2ωj2

) R2 ∑j

cj2

2ωj2

(2.19b)

λET ) ∑j

(cjd - cj

a)2

2ωj2

) (1 - R)2 ∑j

cj2

2ωj2

(2.20)

Jd(ω) ) xπ λGωωG

e-[ω/(2ωG)]2

+ 2λDωωD

ω2 + ωD2

(2.21a)

Ja(ω) ) R2Jd(ω) (2.21b)

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711973

on solvation dynamics and absorption spectra of coumarin 343in water.13,71

D. Observables of Interest and Dynamical Methods.Several observables are of interest for the study of heterogeneousET in dye-semiconductor systems, in particular, the electronicpopulation dynamics, the associated nuclear wave packetdynamics, as well as stationary and time-resolved spectra. Inthis work, we will concentrate on the photoinduced electronicinjection dynamics, which are most directly reflected by thetime-dependent population of the donor state

Here, we have assumed that the system is initially prepared byan ultrafast laser pulse in the donor state|ψd〉. The initial stateof the nuclear degrees of freedom is specified by the Boltzmannoperator e-âHNg of the nuclear Hamiltonian in the electronicground state

To simulate the quantum dynamics of this system, we usethe multilayer (ML) formulation40,72 of the multiconfigurationtime-dependent Hartree (MCTDH) method73-76 in combinationwith an importance sampling scheme to describe the thermalinitial conditions in the observables introduced above. Themethod as well as applications to different reactions in thecondensed phase have been described in detail previously.37,40,77

Here, we only briefly introduce the general idea and give somedetails specific to the application in this work.

The ML-MCTDH method40 is a variational approach for thedescription of quantum dynamics in systems with many degreesof freedom. It extends the original MCTDH method73-76 forapplication to significantly larger systems. In the original (single-layer) MCTDH method, the overall wave function is expandedin terms of time-dependent configurations

Here, |φjkk (t)〉 is the “single-particle” (SP) function for thekthSP degree of freedom, andM denotes the number of SP degreesof freedom. Each SP group usually contains several (Cartesian)degrees of freedom in our calculation, and for convenience theSP functions within the same SP degree of freedom are chosento be orthonormal.

In contrast to the original MCTDH method, where the SPfunctions are represented by time-independent basis functions

the ML-MCTDH method employs adynamiccontraction of thebasis functions that constitute the SP functions. To this end, atime-dependentmulticonfigurational expansion of the SP func-tions is used

i.e., the basic strategy of MCTDH is adopted to treat each SPfunction. Here,Q(k) denotes the number of level two (L2) SPdegrees of freedom in thekth level one (L1) SP group, and|V iqk,q(t)〉 is the L2-SP function for theqth L2-SP degree offreedom. Employing two dynamical layers, the expansion ofthe overall wave function can thus be written in the form

The extension to more dynamical layers is obvious. In thecalculation considered below up to three dynamical layers areemployed.

The equations of motion within the ML-MCTDH approachcan be obtained from the Dirac-Frenkel variational principle.40For two layers, they are given by

where the mean-field operators, reduced densities, and projectionoperators are defined in ref 40. The equations of motion forfurther layers are again obvious extensions of eq 2.28. Theinclusion of several dynamically optimized layers in the ML-MCTDH method provides more flexibility in the variationalfunctional, which significantly advances the capabilities ofperforming wave packet propagations in a complex system. Thishas been demonstrated by several applications to quantumdynamics in the condensed phase including many degrees offreedom.37,40,72,77-80

III. Application to the Dye -Semiconductor SystemCoumarin 343-TiO2

As a representative example of interfacial ET processes, weconsider photoinduced electron injection in the dye-semicon-ductor system coumarin 343 (C343)-TiO2. This system hasbeen investigated experimentally by a number of groups.3,5,6,13,81

Recently, we have studied the electronic injection dynamics aswell as the associated nuclear wave packet dynamics in thissystem employing a semiempirical Newns model.41 Here, weapply the first-principles model outlined above.

A. Characterization of the System, Donor-AcceptorSeparation, and Coupling Matrix Elements.To model C343adsorbed on TiO2 nanoparticles at the atomic level, we haveconsidered complexes of C343 with anatase TiO2 clusters ofdifferent sizes, as depicted in Figure 1. All interatomic distancesand valence angles of the TiO2 clusters were taken from theX-ray structure of bulk anatase.82 To avoid artificial effects dueto dangling bonds, the clusters were saturated by adding

Pd(t) )1

Tr[e-âHNg]Tr[e-âHNg|ψd〉〈ψd|eiHt|ψd〉〈ψd|e-iHt] (2.22)

HNg )1

2∑

l

(Pl2 + Ωl

2Ql2) +

1

2∑

j

(pj2 + ωj

2xj2) (2.23)

|Ψ(t)〉 ) ∑J

AJ(t)|ΦJ(t)〉 ≡

∑j1

∑j2

‚‚‚ ∑jM

Aj1 j2‚‚‚jM(t) ∏k)1

M

|φjkk (t)〉 (2.24)

|φnk(t)〉 ) ∑I

BIk,n(t)|uIk〉 (2.25)

|φnk(t)〉 ) ∑I

BIk,n(t)|uIk(t)〉 ≡

∑i1

∑i2

‚‚‚ ∑iQ(k)

Bi1i2‚‚‚iQ(k)k,n (t) ∏

q)1

Q(k)

|Viqk,q(t)〉 (2.26)

|Ψ(t)〉 ) ∑j1

∑j2

‚‚‚ ∑jM

Aj1 j2‚‚‚jM(t)

× ∏k)1

M

[∑i1

∑i2

‚‚‚ ∑iQ(k)

Bi1i2 ‚‚‚ iQ(k)k, jk (t) ∏

q)1

Q(k)

|V iqk,q(t)〉] (2.27)

i|Ψ̇(t)〉L1 coefficients) Ĥ(t)|Ψ(t)〉 (2.28a)

i|φk(t)〉L2 coefficients)[1 - P̂k(t)][ F̂k(t)]-1〈Ĥ(t)〉k|φk(t)〉 (2.28b)

i|ν̆k,q(t)〉L3 coefficients)[1 - P̂L2

k,q(t)][ F̂k,q(t)]-1〈Ĥ (t)〉k,q|Vk,q(t) (2.28c)

11974 J. Phys. Chem. C, Vol. 111, No. 32, 2007 Kondov et al.

hydrogen atoms and hydroxyl groups to the boundary oxygenand titanium atoms, respectively. The number of added hydrogenatoms and hydroxyl groups as well as the adsorption sites werechosen in a way to obtain neutral closed-shell clusters with highcoordination of the boundary titanium and oxygen atoms. Verysimilar saturated cluster models have been used to study surfacephotoreactions on anatase nanoparticles83 as well as adsorptionof water and catechol on the (101) anatase surface.84 Theadsorption site of the clusters is characterized by two titaniumatoms from the (101) surface of anatase (see below). Theminimal model that can capture all of these features is the cluster(TiO2)2(H2O)5 (Figure 1, left image). However, significantlylarger clusters had to be considered to minimize boundaryeffects. Well converged results could be obtained with the cluster(TiO2)24(H2O)30, and only these results will be reported in thefollowing.

To obtain the structure of the C343-(TiO2)24(H2O)30 complexshown in Figure 1 (right image) we have used the followingprotocol: The geometry of isolated C343 was taken from anearlier study.42 The deprotonated form of C343 was aligned tothe saturated (TiO2)8(H2O)14 cluster (Figure 1, middle image)by optimizing the ground-state energy in internal coordinates.Thereby, the internal nuclear degrees of freedom of C343 andof the cluster were kept fixed, and only the six relativeorientation coordinates (three translations and three rotations)were allowed to vary. Then, C343 was attached to the larger(TiO2)24(H2O)30 cluster (Figure 1, right image) using the sixrelative orientation coordinates from the alignment optimizationat the smaller (TiO2)8(H2O)14 cluster. The proton detached fromC343 upon adsorption was attached to a surface oxygen atomadjacent to the adsorption center. This choice of the protocoland the adsorption site is supported by a more detailed electronicstructure study on the adsorption of C343 on anatase TiO2,85

which has revealed that (i) the adsorbate is deprotonated uponadsorption and the proton is attached to a doubly coordinatedsurface oxygen atom and (ii) the preferred complexation isbidentate bridging as shown in Figure 1 but not bidentatechelation to only one surface titanium atom.

The alignment of C343 relative to the cluster (TiO2)8(H2O)14was optimized with DFT usingGaussian 0386 with the B3LYPfunctional and the 3-21G basis set. All other electronic structure

calculations were performed with the program package TUR-BOMOLE87 employing DFT with the B3LYP functional andthe SV(P) basis set.

To discuss the donor-acceptor partitioning procedure, wefirst consider the energy-level scheme. Figure 2 shows theenergies of the molecular orbitals of the overall system as wellas those of the donor and acceptor orbitals obtained by thepartitioning procedure outlined in section IIB. Also shown, incomparison, are the energy levels of the isolated (TiO2)24(H2O)30cluster and the isolated chromophore C343. The isolated(TiO2)24(H2O)30 cluster exhibits a rather dense level structurewith a valence and conduction band separated by a band gap.The calculated value for band gap of the finite cluster is 2.8eV, which is somewhat smaller than calculated (4.0 eV88) andexperimental (3.4 eV89) values for anatase TiO2 nanoparticles.This underestimation of the band gap is presumably due to theadded hydrogen and hydroxyl groups used to saturate the cluster.Unsaturated finite clusters88 show typically a larger band gap

Figure 1. Complexes of C343 with the clusters (TiO2)2(H2O) (left image), (TiO2)8(H2O)14 (middle image), and (TiO2)24(H2O)30 (right image).

Figure 2. Representation of the energy levels of the system investi-gated. Shown are (from left to right) energy levels of the isolatedchromophore C343, the donor molecular orbitals,|æj nd〉, as obtainedfrom the partitioning procedure, the complex (TiO2)24(H2O)30C343, theacceptor molecular orbitals,|æj na〉, as obtained from the partitioningprocedure, and the pure cluster (TiO2)24(H2O)30. The orbital chosen asthe donor state is denoted by|Ψd〉. Furthermore, correlations betweenselected energy levels are indicated.

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711975

than bulk anatase. A detailed analysis of the orbitals of (TiO2)24-(H2O)30 revealed that the lowest unoccupied orbitals arelocalized predominantly on saturation groups (cf. Figure 2,rightmost panel) and can be regarded as levels in the band gap.As has been demonstrated in a computational study of similarclusters,83 this deficiency of the saturated cluster model is notexpected to have a significant influence on the electronic levelsinvolved in ET transitions. Moreover, these levels in the bandgap do not couple to the donor levels of C343 in the complex(see below).

The adsorption of the chromophore C343 on the (TiO2)24-(H2O)30 cluster changes the level structure noticeably. Inparticular, it introduces energy levels in the lower part of theband gap, which can be associated with the highest occupiedmolecular orbitals (in particular HOMO and HOMO- 2) ofthe isolated chromophore. The complex also exhibits a fewenergy levels in the higher part of the band gap, which

correspond to orbitals localized at the TiO2 cluster. While thehighest occupied levels of C343 are located in the band gapand thus retain their discrete structure in the complex, the lowestunoccupied levels of C343 (in particular LUMO and LUMO+1) are located energetically in the conduction band of TiO2. Asa consequence, in the complex these levels are dissolved in thedense manifold of conduction band levels.

The partitioning procedure results in orbitals localized at thechromophore and the TiO2 cluster, respectively. Although theenergy levels of both parts resemble the level structure ofisolated C343 and TiO2 to some extent, there are noticeabledifferences due to the fact that these orbitals are not themolecular orbitals of the separated parts but take some of theinteraction into account. For the study of electron-injectiondynamics, the donor orbital is chosen as the orbital thatcorresponds in the limit of infinite separation to the LUMO ofisolated C343. Employing TD-DFT calculations, it has been

Figure 3. Selected orbitals obtained with the partitioning procedure. Shown are the orbitals corresponding to the HOMO orbital of isolated C343(A), the donor orbital (B), and two representative acceptor orbitals (C and D).

11976 J. Phys. Chem. C, Vol. 111, No. 32, 2007 Kondov et al.

shown recently42 that this orbital is the dominant excitation inisolated C343 and in complexes with small clusters of TiO2.90

The acceptor orbitals include all orbitals localized at the TiO2cluster with energies above the energy of the HOMO of theoverall system.

The local character of the orbitals resulting from the partition-ing procedure is illustrated in Figure 3. The orbital that can beassociated to the HOMO orbital of isolated C343 (in thecomplex, this orbital corresponds to HOMO- 1) as well asthe donor orbital are well localized on the chromophore. Theacceptor orbitals are, however, localized at the TiO2 cluster.The latter orbitals are dominated by the 3d orbitals of titanium.

In the system investigated, the localization works very wellfor all donor and acceptor orbitals that participate in the ETprocess. In the energy range of interest, the maximal nonlocalcontribution to donor or acceptor states is about 1%. It shouldbe emphasized, however, that the localization method (as anylocalization procedure) should be tested for each system to whichit is applied. In the method used here, problems may arisebecause due to the orthogonalization, which precedes thedonor-acceptor separation, some of the local character of theorbitals may be lost. This concerns in particular orbitals localizedclose to the dye-semiconductor binding site. An example ofsuch an orbital is shown in Figure 4. Although this orbital ispredominantly localized at C343 it also has non-negligiblecontributions from the TiO2 cluster. However, this orbitalcorresponds to an occupied orbital of the overall system, withan energy well separated from the donor state, and is thus notinvolved in the electron-injection process.

The donor-acceptor coupling matrix elements obtained basedon the partitioning are depicted in Figure 5. It is seen that a

rather broad distribution of acceptor states couples to the donorstate. In contrast to the Newns model used in our previousstudy,41 where the donor-acceptor coupling varies smoothlywith the energy�k, the first-principles-based couplings exhibitsignificant structures.

B. Electron-Transfer Dynamics. On the basis of the first-principles model discussed above, we have performed dynamicalsimulations of the ET dynamics. Thereby, the chosen donorstate, all 1184 acceptor states, and 39 modes of C343 (selectedaccording to their electronic-vibrational coupling strength) weretaken into account explicitly. The continuous distribution ofsolvent modes was represented by 20 additional oscillators.

Figure 6 shows the result of the simulation for the populationof the donor state after photoexcitation (thick dashed line). Thesimulation predicts an ultrafast injection of the electron fromthe donor state localized at the chromophore into the quasi-continuum of acceptor states localized in the TiO2 cluster on atime scale (1/e time) of ∼13 fs. In addition to the ultrafastinjection component, the simulation results also exhibit a smallcomponent of slower injection dynamics as well as oscillatorystructures superimposed on the decay. A comparison with apurely electronic calculation (thin dashed line in Figure 6), wherethe coupling to the nuclear degrees of freedom has been set tozero, reveals that the high-frequency oscillations are of electronicorigin, i.e., can be classified as electronic coherence. In theresults of the purely electronic calculation, these coherenceeffects are much more pronounced than in the full vibronicresults (thick dashed line in Figure 6). Thus, the coupling to

Figure 4. Example of a “donor” orbital, where the orthogonalizationprocedure results in noticeable contributions at the TiO2 cluster

Figure 5. Modulus of the donor-acceptor coupling matrix elementsVdk. The red line indicates the energy of the donor level,�d.

Figure 6. Population dynamics of the donor state after photoexcitation.Shown are results obtained with vibronic coupling (thick lines), withoutvibronic coupling (thin lines), for the finite TiO2 cluster (dashed lines),and for the model of an infinite TiO2 surface (solid lines).

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711977

the nuclear degrees of freedom results in a significant deco-herence effect. In addition to this quenching of electroniccoherence, the coupling to the nuclear degrees of freedom alsointroduces slower oscillations of vibrational origin. This vibra-tional coherence effect is, however, small in the present system.

The results in Figure 6 also show that the electron-injectionprocess is not complete: There is a small but noticeableprobability (∼2%) to find the electron for long times at the donorstate. This finite probability for electron trapping at the donoralso persists for even longer times (data not shown). Theincomplete injection is a result of the finite cluster considered.If an additional imaginary part (σ ) 1 eV) is included into theorbital energies of the outer atoms of the TiO2 cluster (cf. thediscussion in section IIB and the Appendix) to mimic electroninjection at an infinite surface, then the donor population decaysto zero. This is demonstrated by the solid lines in Figure 6.The result for the infinite system agrees well with the one forthe finite TiO2 cluster for short times but decays to zero forlonger times, corresponding to a complete electron-injectionprocess.

The time scale of electron injection predicted by the simula-tion (∼13 fs) is faster than the experimental results for theC343-TiO2 system, where injection times in the range of 20-200 fs have been found using different techniques.3,5,6,13,81Thisdiscrepancy can have a variety of reasons. As discussed above,the electron-injection dynamics are not a single-exponentialdecay but also exhibit a slower injection component as well asoscillatory structures, which may result effectively in an overalllonger injection time. Furthermore, the dynamics depend on theenergy-level structure, in particular the relative position of thedonor state with respect to the conduction band edge, as wellas on the donor-acceptor coupling matrix elements and thuson the accuracy of the electronic structure model used. Anotherreason for the deviation may be the limited time resolution ofthe experiments.

Finally, Figure 7 shows a comparison of results obtained fromthe first-principles model, where the electronic energies andelectronic coupling matrix elements have been determined byelectronic structure calculations, with results where theseparameters have been determined by the semiempirical Newnsmodel.41 Overall, the two models predict similar ET character-istics and thus confirm the robustness of the Newns model. Themajor differences are the slower ultrafast injection component(by about a factor of 2) and the electronic coherences in the

result based on the first-principles model. The different ET timescale is caused by the overall stronger donor-acceptor couplingin the semiempirical Newns model. The different importanceof electronic coherence effects, however, is related to the waythe donor-acceptor coupling is described in the two models.In the semiempirical Newns model the donor-acceptor couplingmatrix elementsVdk are described by a continuous functionΓ(E) (cf. the discussion in the Appendix). Because in the modelused the functionΓ(E) varies slowly and, furthermore, theenergy of the donor state is well above the conduction bandedge of the semiconductor,41 the result of the Newns modeldoes not show electronic coherence effects. In the first-principlesmodel, however, the donor-acceptor coupling matrix elementsVdk depend significantly on the energy�k, thus resulting inpronounced electronic coherence effects in the populationdynamics. The comparison in Figure 7 also shows that the effectof the coupling to the nuclear degrees of freedom on theelectron-injection time scale is more pronounced in the semiem-pirical Newns model.

IV. Concluding Remarks

In this paper, we have outlined a first-principles-based methodto describe the quantum dynamics of heterogeneous ET reactionsat dye-semiconductor interfaces. The method employs anexpansion of the Hamiltonian in a diabatic basis of electronicdonor and acceptor states localized at the dye molecule and thesemiconductor substrate, respectively. To determine the diabaticstates and thus the electronic energies and the donor-acceptorcoupling matrix elements, we have used a partitioning scheme.This scheme is based on a partitioning of the overall Hilbertspace into a donor and acceptor part and a subsequent separatediagonalization of the two blocks of the Hamiltonian to definethe donor and acceptor states. In this article, we have employedthe Kohn-Sham orbitals and matrix to describe the system andthus used an effective single-electron Hamiltonian. The exten-sion of the method to many-electron states will be the subjectof future work.

As an application, we have considered photoinduced electroninjection for coumarin 343 adsorbed at titanium oxide nano-particles. The latter were modeled by a finite titanium oxidecluster. The quantum dynamics of the ET reaction weresimulated using the ML-MCTDH method, which allows anefficient and accurate description of this system, which com-prises many electronic states and nuclear degrees of freedom.The results demonstrate the ultrafast character of the electron-injection process in this system. The ET dynamics exhibitsignificant electronic coherence effects. The coupling to thenuclear degrees of freedom of the chromophore results in aquenching of the coherence effects.

In the present application we have assumed that the photo-excitation by an ultrashort laser pulse can be described by aninstantaneous transition from the electronic ground state to thedonor state. As shown previously,72 the methodology also allowsus to include the laser field explicitly in the calculation to studythe influence of the laser pulse on the dynamics of these ultrafastET reactions. Employing, furthermore, the nonperturbativedescription of matter-field interaction outlined recently,80,91it will also be possible to simulate time-resolved nonlinearspectra, which will allow a direct comparison with experimentalresults.

Appendix

Description of Electron Injection for a ChromophoreAdsorbed on an Extended Substrate.As mentioned above,

Figure 7. Population dynamics of the donor state after photoexcitationobtained by employing the first-principles-based model (solid lines)and the semiempirical model for the electronic coupling (dashed lines).Fully vibronic and purely electronic population dynamics are depictedby thick lines and thin lines, respectively.

11978 J. Phys. Chem. C, Vol. 111, No. 32, 2007 Kondov et al.

the partitioning procedure introduced in section IIB is not limitedto dye-semiconductor systems with a finite semiconductorcluster but can, in principle, also be applied to a dye moleculeadsorbed on an extended surface. One possibility is to employthe slab model and electronic structure calculations with periodicboundary conditions.92 Alternatively, the effect of an infinitesemiconductor substrate can also be described using surfaceGreen’s function techniques.59 In this appendix, we outline anapproximate variant of the latter method.

To this end, let us assume that the partitioning procedureoutlined in section IIB has been performed for a chromophoreadsorbed on an infinite surface (e.g., using the slab model)resulting in a Hamiltonian of the form of eq 2.1. We first showthat if one is only interested in observables that are localizedon the chromophore, then the influence of the semiconductorsubstrate and the chromophore surface coupling on the dynamicsis fully characterized by the function

or, equivalently, its Fourier transform

The latter function describes the density of states of thesemiconductor substrate weighted by the donor-acceptorcoupling and is also called the energy-dependent decay widthof the donor state.

To demonstrate this fact, let us consider the electronicprojection of the time-dependent vibronic wave function

onto the donor state

where|Ψ0〉 denotes the initial state and the HamiltonianH isgiven by eq 2.15. In the following, we will assume that theinitial wave function is localized at the chromophore, i.e.,

Using projection-operator techniques, it is straightforwardto show53 that the equation of motion for〈ψd|Ψ(t)〉 isgiven by

where

denotes the nuclear Hamiltonian in the donor state and

is the nuclear Hamiltonian in the acceptor states. Equation A.6shows that the influence of the semiconductor substrate and ofthe chromophore-surface coupling enters only through thefunction Γ(t) or, equivalently, its Fourier transformΓ(E).

While Γ(t) is a smooth function for finite semiconductorclusters and extended surfaces,Γ(E) is a continuous functiononly for a chromophore adsorbed on an infinite surface. Thewidth functionΓ(E) is the imaginary part of the self-energy inthe donor stateΣdd(E)

where

describes the interaction between the chromophore and thesemiconductor surface and

is the electronic Green’s function of the semiconductor surface.Thereby,Hsf denotes the electronic Hamiltonian of the semi-conductor substrate andη is the usual positive infinitesimal.

In our previous work on heterogeneous ET37,41we have useda semiempirical Newns model, whereΓ(E) was parametrizedbased on a tight-binding model developed by Petersson et al.43

The parameters within this model have been determined to fitthe lower 3d group of the TiO2 conduction band (see refs 41and 43 for further details).

As was mentioned above, a first-principles calculation ofΓ(E) is possible by employing the slab model and electronicstructure calculations with periodic boundary conditions. Al-ternatively, a finite part of the semiconductor surface (in thefollowing referred to as the cluster) can be treated explicitly,and the influence of the remaining infinite part can be describedusing surface Green’s function techniques.59 Within this methodthe effect of the infinite substrate enters via a self-energy matrixthat is localized at the boundary of the cluster, which is treatedexplicitly. To discuss this approach, we introduce a projectionoperatorP that projects on the cluster, i.e., on the part of thesubstrate that is explicitly treated. Using standard projection-operator techniques one obtains for the projected Green’sfunction of the surface

Here,M(E) is a self-energy term that describes the influence ofthe remainder of the substrate given by

whereQ ) 1 - P. The self-energyM(E) in eq A.13 should notbe confused with the self-energyΣ(E) defined in eq A.9b. Whilethe latter describes the influence of the overall substrate on theadsorbate, the former describes the effect of the remaining partof the infinite substrate, without the explicitly treated TiO2

Γ(t) ) ∑k

|Vdk|2 e-i�kt (A.1)

Γ(E) ) 2π ∑k

|Vdk|2δ(E - �k) (A.2)

|Ψ(t)〉 ) e-iHt|Ψ0〉 (A.3)

〈ψd|Ψ(t)〉 ) 〈ψd| e-iHt|Ψ0〉 (A.4)

〈ψk|Ψ0〉 ) 0 (A.5)

∂

∂t〈ψd|Ψ(t)〉 )

-iHNd〈ψd|Ψ(t)〉 - ∫0t dτ Γ(τ) e-iHNaτ〈ψd|Ψ(t - τ)〉 (A.6)

HNd ) 〈ψd|H|ψd〉

) �d +1

2∑

l

(Pl2 + Ωl

2Ql2) + ∑

l

κldQl +

1

2∑

j

(pj2 + ωj

2xj2) + ∑

j

cjdxj (A.7)

HNa )1

2∑

l

(Pl2 + Ωl

2Ql2) +

∑l

κlaQl +

1

2∑

j

(pj2 + ωj

2xj2) + ∑

j

cjaxj (A.8)

Γ(E) ) -2 Im Σdd(E) (A.9a)

Σ dd(E) ) 〈ψd|VGsf(E)V|ψd〉 (A.9b)

V ) ∑k

(|ψd〉Vdk〈ψk| + |ψk〉Vkd〈ψd|) (A.10)

Gsf(E) ) (E + iη - Hsf)-1 (A.11)

PGsf(E)P ) (E + iη - PHsfP - M(E))-1 (A.12)

M(E) ) PHsfQ(E + iη - QHsfQ)-1QHsfP (A.13)

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711979

cluster, on the explicitly treated system, i.e., the complex ofthe dye molecule and the finite TiO2 cluster.

Within our treatment outlined in section IIB the projectionoperatorP is given by the orthogonal orbitals of the explicitlytreated acceptor space

and the projected Hamiltonian of the substrate,PHsfP, is givenby the Fock matrix of the acceptor space in the orthogonal basis

In principle, the energy-dependent self-energy matrixM(E)can be calculated using surface Green’s function techniques.In the application considered in this paper, we have used avariant of this method, which approximates the self-energy bya constant diagonal imaginary partσ at the outer atoms of theexplicitly treated TiO2 cluster; i.e.,M(E) ≈ M with Mjj ) -iσ/2if j belongs to an orbital of the outer atoms of the TiO2 cluster,andMjk ) 0 otherwise. Thus, within this method the acceptorblock of the Fock matrix from eq 2.5 is replaced by

As a result, the Fock matrix is no longer real but complexsymmetric.

In our practical implementation, we calculateΓ(E) via therelation to the self-energyΣdd(E), eq A.9a, with

Here,Gaa denotes the matrix representation ofPGsf(E)P in theorthogonal basis|æ̃na〉

The matrix F̃′da is obtained by diagonalizing the donor blockF̃dd according to eq 2.7 and transforming the off-diagonal blocksaccording toF̃′da ) Dd

†F̃da. Furthermore, in eq A.17, we haveassumed thatQV|ψd〉 ) 0, which is expected to be a very goodapproximation for the size of the TiO2 cluster employed in thepresent study.

To determineGaa, we calculate the right eigenvectors andeigenvalues of the complex symmetric matrixF̃aa + M.Denoting the matrix of right eigenvectors byU and the diagonalmatrix of eigenvalues byλ and using the identitiesF̃′†da ) F̃′daand UW-1UT ) 1, whereW ) UTU is the overlap of theeigenvectors ofF̃aa + M, we obtain the energy-dependent decaywidth for the selected donor state

Alternatively, the Green’s functionGaa could also be determineddirectly for each energyE using, e.g., matrix inversion.However, in the present context, the diagonalization procedureemployed is more advantageous because it has to be performedonly once.

In the dynamical simulations, the continuum of electronicstates implicit in the continuous functionΓ(E) is discretizedand represented by a finite number of states|ψk〉 employing eq

A.2 as described previously.37 In the present applications, 6000electronic states within an equidistant discretization schema weresufficient to represent the electronic continuum over the timescale of interest.

Acknowledgment. We thank Wolfgang Domcke for numer-ous helpful discussions. The generous allocation of computingtime by the National Energy Research Scientific ComputingCenter and the Leibniz Rechenzentrum, Munich, is gratefullyacknowledged. This work has been supported by the DeutscheForschungsgemeinschaft (DFG) through the DFG-Cluster ofExcellence Munich-Centre for Advanced Photonics and aresearch grant (M.T.), the Fonds der Chemischen Industrie (MT),the National Science Foundation CAREER award CHE-0348956(H.W.), the Alexander von Humboldt foundation, and researchgrant GACR 202/07/0833 (M.C.).

References and Notes

(1) Moser, J. E.; Gra¨tzel, M. Chem. Phys.1993, 176, 493.(2) Hagfeldt, A.; Gra¨tzel, M. Chem. ReV. 1995, 95, 49.(3) Rehm, J. M.; McLendon, G. L.; Nagasawa, Y.; Yoshihara, K.;

Moser, J.; Gra¨tzel, M. J. Phys. Chem.1996, 100, 9577.(4) Martini, I.; Odak, J.; Hartland, G. V.; Kamat, P. V.J. Chem. Phys.

1997, 107, 8064.(5) Gosh, H. N.; Asbury, J. B.; Wang, Y.; Lian, T.J. Phys. Chem. B

1998, 102, 10208.(6) Wachtveitl, J.; Huber, R.; Spo¨rlein, S.; Moser, J.; Gra¨tzel, M. Int.

J. Photoenergy1999, 1, 153.(7) Willig, F.; Zimmermann, C.; Ramakrishna, S.; Storck, W.Elec-

trochim. Acta2000, 45, 4565.(8) Zimmermann, C.; Willig, F.; Ramakrishna, S.; Burfeindt, B.;

Pettinger, B.J. Phys. Chem. B2001, 105, 9245.(9) Asbury, J.; Hao, E.; Wang, Y.; Ghosh, H. N.; Lian, T.J. Phys.

Chem. B2001, 105, 4545.(10) Ramakrishna, G.; Gosh, H. N.J. Phys. Chem. A2002, 106, 2545.(11) Schnadt, J.; Bru¨hwiler, P. A.; Patthey, L.; O’Shea, J. N.; So¨dergreen,

S.; Odellus, M.; Ahuja, R.; Karis, O.; Ba¨ssler, M.; Persson, P.; Siegbahn,H.; Lunell, S.; Martenson, N.Nature2002, 418, 620.

(12) Walters, K. A.; Gaal, D. A.; Hupp, J. T.J. Phys. Chem. B2002,106, 5139.

(13) Huber, R.; Moser, J. E.; Gra¨tzel, M.; Wachtveitl, J.Chem. Phys.2002, 285, 39.

(14) Huber, R.; Moser, J. E.; Gra¨tzel, M.; Wachtveitl, J.J. Phys. Chem.B 2002, 106, 6494.

(15) Kallioinen, J.; Benko¨, G.; Sundstro¨m, V.; Korrpi-Tommola, J.;Yartsev, A.J. Phys. Chem. B2002, 106, 4396.

(16) Takeshita, K.; Sasaki, Y.; Kobashi, M.; Tanaka, Y.; Maeda, S.;Yamakata, A.; Ishibashi, T.; Onishi, H.J. Phys. Chem. B2003, 107, 4156.

(17) Wang, L.; Ernstorfer, R.; Willig, F.; May, V.J. Phys. Chem. B2005, 109, 9589.

(18) Hagfeldt, A.; Gra¨tzel, M. Acc. Chem. Res.2000, 33, 269.(19) Grätzel, M. Nature2001, 414, 338.(20) Benkö, G.; Kallioinen, J.; Korppi-Tommola, J.; Yartsev, A.;

Sundstro¨m, V. J. Am. Chem. Soc.2002, 124, 489.(21) Stier, W.; Prezhdo, O.Isr. J. Chem.2002, 42, 213.(22) Stier, W.; Prezhdo, O.J. Phys. Chem. B2002, 106, 8047.(23) Stier, W.; Prezhdo, O.AdV. Mater. 2004, 16, 240.(24) Duncan, W.; Stier, W.; Prezhdo, O.J. Am. Chem. Soc.2005, 127,

7941.(25) Duncan, W.; Stier, W.; Prezhdo, O.J. Phys. Chem. B2005, 109,

365.(26) Rego, L.; Batista, V.J. Chem. Phys.2005, 122, 154709.(27) Newns, D.Phys. ReV. 1969, 178, 1123.(28) Ramakrishna, S.; Willig, F.; May, V.Phys. ReV. B 2000, 62, 16330.(29) Ramakrishna, S.; Willig, F.J. Phys. Chem. B2000, 104, 68.(30) Ramakrishna, S.; Willig, F.; May, V.J. Chem. Phys.2001, 115,

2743.(31) Schreiber, M.; Kondov, I.; Kleinekatho¨fer, U. J. Lumin.2001, 94,

471.(32) Ramakrishna, S.; Willig, F.; May, V.Chem. Phys. Lett.2002, 351,

242.(33) Ramakrishna, S.; Willig, F.; May, V.J. Phys. Chem. B2003, 107,

607.(34) Wang, L.; May, V.J. Chem. Phys.2004, 121, 8039.(35) Liang, K.; Lin, C.-K.; Chang, H.-C.; Lin, S.J. Chem. Phys.2006,

125, 154706.(36) Wang, L.; Willig, F.; May, V.J. Chem. Phys.2006, 124, 014712.(37) Thoss, M.; Kondov, I.; Wang, H.Chem. Phys.2004, 304, 169.

P ) ∑n

|æ̃na〉〈æ̃na| (A.14)

〈æ̃na|PHsfP|æ̃ma 〉 ) F̃aa,nm (A.15)

F̃aa f F̃aa + M (A.16)

Σdd ) 〈ψd|VGsf(E)V|ψd〉) 〈ψd|VPGsf(E)PV|ψd〉) F̃′daGaa(F̃′da)

† (A.17)

Gaa,nm ) 〈æ̃na|PGsf(E)P|æ̃ma 〉 (A.18)

Γ(E) ) -2 Im{F̃′daU 1W(E - λ) UTF̃′ad} (A.19)

11980 J. Phys. Chem. C, Vol. 111, No. 32, 2007 Kondov et al.

(38) Wang, H.; Thoss, M.; Miller, W. H.J. Chem. Phys.2001, 115,2979.

(39) Wang, H.; Thoss, M.Isr. J. Chem.2002, 42, 167.(40) Wang, H.; Thoss, M.J. Chem. Phys.2003, 119, 1289.(41) Kondov, I.; Thoss, M.; Wang, H.J. Phys. Chem. A2006, 110,

1364.(42) Kondov, I.; Wang, H.; Thoss, M.Int. J. Quantum Chem.2006,

106, 1291.(43) Petersson, A.; Ratner, M.; Karlsson, H.J. Phys. Chem. B2000,

104, 8498.(44) Mulliken, R.J. Am. Chem. Soc.1952, 74, 811.(45) Hush, N.Prog. Inorg. Chem.1968, 13, 1005.(46) Cave, R.; Newton, M.Chem. Phys. Lett.1996, 249, 15.(47) Cave, R.; Newton, M.J. Chem. Phys.1997, 106, 9213.(48) Voityuk, A.; Rösch, N.J. Chem. Phys.2000, 117, 5607.(49) For an overview, see, for example, ref 93 and references therein.(50) Feshbach, H.Ann. Phys.1962, 19, 287.(51) O’Malley, T. Phys. ReV. 1967, 162, 98.(52) Domcke, W.Phys. ReV. A 1983, 28, 2777.(53) Domcke, W.Phys. Rep.1991, 208, 97.(54) Similar partitioning methods have been used in variety of other

fields, for example, in the context of electron transport through singlemolecule junctions.94 Particularly closely related to the approach used hereis the method employed in ref 60.

(55) Kurnikov, L.; Beratan, D.J. Chem. Phys.1996, 105, 9561.(56) Galperin, M.; Toledo, S.; Nitzan, A.J. Chem. Phys.2002, 117,

10817.(57) Löwdin, P.-O.J. Chem. Phys.1950, 18, 365.(58) Mayer, I.Int. J. Quantum Chem.2002, 90, 63.(59) Xue, Y.; Ratner, M.Phys. ReV. B 2001, 68, 115406.(60) Benesch, C.; Cizek, M.; Thoss, M.; Domcke, W.Chem. Phys. Lett.

2006, 430, 355.(61) This correponds to the Condon approximation, which is often

employed in ET systems, and is expected to be valid for the relatively rigidsystems considered here.

(62) Dushinski, F.; Sassetti, M.; Weiss, U.Acta Physicochim. URSS1937, 7, 551.

(63) Myers, A.Chem. ReV. 1996, 96, 911.(64) Conical Intersections: Electronic Structure, Dynamics and Spec-

troscopy; Domcke, W., Yarkony, D. R., Ko¨ppel, H., Eds.; World Scien-tific: Singapore, 2004.

(65) Marcus, R. A.; Sutin, N.Biochim. Biophys. Acta1985, 811, 265.(66) Weiss, U.Quantum DissipatiVe Systems, 2nd ed.; World Scien-

tific: Singapore, 1999.(67) Makri, N. J. Phys. Chem. B1999, 103, 2823.(68) Georgievskii, Y.; Hsu, C.-P.; Marcus, R. A.J. Chem. Phys.1999,

110, 5307.(69) Rips, I.; Jortner, J.J. Chem. Phys.1987, 87, 2090.(70) May, V.; Kühn, O. Charge and Energy Transfer Dynamics in

Molecular Systems: A Theoretical Introduction; Wiley-VCH: Berlin, 2000.(71) Jimenez, R.; Fleming, G. R.; Kumar, P. V.; Maroncelli, M.Nature

1994, 369, 471.(72) Wang, H.; Thoss, M.J. Chem. Phys.2006, 124, 034114.(73) Meyer, H.-D.; Manthe, U.; Cederbaum, L. S.Chem. Phys. Lett.

1990, 165, 73.(74) Manthe, U.; Meyer, H.-D.; Cederbaum, L. S.J. Chem. Phys.1992,

97, 3199.

(75) Beck, M. H.; Ja¨ckle, A.; Worth, G. A.; Meyer, H.-D.Phys. Rep.2000, 324, 1.

(76) Meyer, H.-D.; Worth, G. A.Theor. Chem. Acc.2003, 109, 251.(77) Thoss, M.; Wang, H.Chem. Phys.2006, 322, 210.(78) Wang, H.; Thoss, M.J. Phys. Chem. A2003, 107, 2126.(79) Thoss, M.; Domcke, W.; Wang, H.Chem. Phys.2004, 296, 217.(80) Wang, H.; Thoss, M.Chem. Phys. Lett.2004, 389, 43.(81) Murakoshi, K.; Yanagida, S.; Capel, M.; Castner, E. Interfacial

electron transfer dynamics of photosensitized zinc oxide nanoclusters. InNanostructured Materials: Clusters, Composites, and Thin Films; Chalaev,V. M., Moskovits, M.. Eds.; ACS Symposium Series 679; AmericanChemical Society: Washigton, DC, 1997; pp 221-238.

(82) Burdett, J. K.; Hughbanks, T.; Miller, G. J.; Richardson, J. W., Jr.;Smith, J. V.J. Am. Chem. Soc.1987, 109, 3639.

(83) Bredow, T.; Jug, K.J. Phys. Chem.1995, 99, 285.(84) Redfern, P. C.; Zapol, P.; Curtiss, L. A.; Rajh, T.; Thurnauer, M.

C. J. Phys. Chem. B2003, 107, 11419.(85) Kondov, I.; Markmann, A.; Thoss, M., to be submitted for

publication.(86) Frisch, M. J.; Trucks, G. W.; Schlegel, H. B.; Scuseria, G. E.; Robb,

M. A.; Cheeseman, J. R.; Montgomery, J. A., Jr.; Vreven, T.; Kudin, K.N.; Burant, J. C.; Millam, J. M.; Iyengar, S. S.; Tomasi, J.; Barone, V.;Mennucci, B.; Cossi, M.; Scalmani, G.; Rega, N.; Petersson, G. A.;Nakatsuji, H.; Hada, M.; Ehara, M.; Toyota, K.; Fukuda, R.; Hasegawa, J.;Ishida, M.; Nakajima, T.; Honda, Y.; Kitao, O.; Nakai, H.; Klene, M.; Li,X.; Knox, J. E.; Hratchian, H. P.; Cross, J. B.; Bakken, V.; Adamo, C.;Jaramillo, J.; Gomperts, R.; Stratmann, R. E.; Yazyev, O.; Austin,A. J.; Cammi, R.; Pomelli, C.; Ochterski, J. W.; Ayala, P. Y.; Morokuma,K.; Voth, G. A.; Salvador, P.; Dannenberg, J. J.; Zakrzewski, V. G.;Dapprich, S.; Daniels, A. D.; Strain, M. C.; Farkas, O.; Malick, D. K.;Rabuck, A. D.; Raghavachari, K.; Foresman, J. B.; Ortiz, J. V.; Cui, Q.;Baboul, A. G.; Clifford, S.; Cioslowski, J.; Stefanov, B. B.; Liu, G.;Liashenko, A.; Piskorz, P.; Komaromi, I.; Martin, R. L.; Fox, D. J.; Keith,T.; Al-Laham, M. A.; Peng, C. Y.; Nanayakkara, A.; Challacombe, M.;Gill, P. M. W.; Johnson, B.; Chen, W.; Wong, M. W.; Gonzalez, C.;Pople, J. A.Gaussian 03, revision B.04; Gaussian, Inc.: Wallingford, CT,2003.

(87) Ahlrichs, R.; Ba¨r, M.; Häser, M.; Horn, H.; Ko¨lmel, C.Chem. Phys.Lett. 1989, 162, 165.

(88) Nilsing, M.; Lunell, S.; Persson, P.; Ojama¨e, L. Surf. Sci.2005,582, 49.

(89) Kormann, C.; Bahnemann, D.; Hoffmann, M.J. Phys. Chem.1988,92, 5196.

(90) It is also noted that the first exited state of isolated C343 correspondsalmost exclusively to a HOMO-LUMO excitation. The excitation energyof 3.43 eV (employing TD-DFT at the B3LYP/SV(P) level) is in goodagreement with the HOMO-LUMO gap (3.59 eV). Therefore, the use ofthe LUMO as a model for the excited state is well justified in this system.

(91) Seidner, L.; Stock, G.; Domcke, W.Chem. Phys. Lett.1994, 228,665.

(92) Nilsing, M.; Persson, P.; Ojama¨e, L. Chem. Phys. Lett.2005, 415,375.

(93) Köppel, H. InConical Intersections: Electronic Structure, Dynam-ics and Spectroscopy; Domcke, W., Yarkony, D. R., H. Ko¨ppel, Eds.; WorldScientific: Singapore, 2004.

(94) Mujica, V.; Kemp, M.; Ratner, M.J. Chem. Phys.1994, 101, 6849.

Dye-Semiconductor Photoinduced ET J. Phys. Chem. C, Vol. 111, No. 32, 200711981

of 12/12

Quantum Dynamics of Photoinduced Electron-Transfer Reactions in Dye-Semiconductor Systems: First-Principles Description and Application to Coumarin 343-TiO 2 Ivan Kondov, ², | Martin C ˇ ı ´z ˇ ek, ‡ Claudia Benesch, ² Haobin Wang,* ,§ and Michael Thoss* ,² Department of Chemistry, Technical UniVersity of Munich, Lichtenbergstrasse 4, D-85747 Garching, Germany, Institute of Theoretical Physics, Faculty of Mathematics and Physics, Charles UniVersity, Prague, Czech Republic, and Department of Chemistry and Biochemistry, MSC 3C, New Mexico State UniVersity, Las Cruces, New Mexico 88003 ReceiVed: March 20, 2007; In Final Form: May 25, 2007 A method to describe the quantum dynamics of photoinduced heterogeneous electron-transfer processes at dye-semiconductor interfaces is proposed. The method is based on a model Hamiltonian, the parameters of which are determined by first-principles electronic structure calculations and a partitioning scheme to define localized donor and acceptor states as well as donor-acceptor coupling matrix elements. On the basis of this modeling procedure, accurate quantum dynamical simulations are performed employing the multilayer multiconfiguration time-dependent Hartree method. As a representative example, applications to coumarin 343 adsorbed on titanium oxide nanoparticles are presented. The results of the simulations show that the ultrafast electron-injection process in this system is accompanied by electronic coherence effects, which are partially quenched due to electronic-nuclear coupling. I. Introduction Photoinduced electron-transfer (ET) reactions at dye- semiconductor interfaces represent an interesting class of ET processes. In particular, the process of electron injection from an electronically excited state of a dye molecule into a semiconductor substrate has been investigated in great detail experimentally in recent years. 1-17 This process represents a key step for photonic energy conversion in nanocrystalline solar cells. 2,6,9,18,19 Employing femtosecond spectroscopy techniques, it has been demonstrated that electron-injection processes at dye-semiconductor interfaces often take place on an ultrafast (sub-picosecond) time scale. 3,8,9,11,13,14,20 For example, electron- injection times as fast as 6 fs have been reported for alizarin adsorbed on TiO 2 nanoparticles 14 in time-resolved experiments, and even faster ET times have been found for biisonicotinic acid on a TiO 2 surface employing resonant photoemission spectroscopy. 11 Other interesting aspects of these ultrafast interfacial ET reactions are the nonequilibrium character and the influence of electronic-nuclear coupling. For example, studies of dye-semiconductor systems with electron-injection time scales on the order of a few tens to a few hundred femtoseconds indicate that the coupling of the electronic dynamics to the nuclear (i.e., vibrational) motion of the chromophore may have a significant impact on the injection process. 8,20 As a result of this correlated electronic-nuclear dynamics, the electron injection in these systems is often not a simple exponential decay process and thus cannot be character- ized by a single rate constant. The theoretical study of such interfacial ET processes requires a quantum mechanical description of the electron-injection dynamics including the coupling to the nuclear degrees of freedom. Since it is currently not feasible to carry out a full quantum dynamical simulation of the interfacial ET dynamics that takes into account the coupling to the nuclear degrees of freedom and employs an adequate electronic structure theory, different approximate strategies have been applied. One pos- sibility is to use a first-principles electronic structure method to describe the dye-semiconductor system but employ an approximate treatment of the nuclear motion. An example is ab initio molecular dynamics, where the dynamics of the nuclear degrees of freedom are described classically. 21-26 Another strategy, which is particularly useful if an accurate, fully quantum dynamical treatment is required, is to use a physically motivated model. A commonly used model to study heteroge- neous ET processes at interfaces is the Anderson-Newns model. 27 Along this line, several workers have studied the electron-injection dynamics based on models of reduced di- mensionality, taking into account typically a single reaction mode. 17,28-36 Dissipative effects, such as vibrational relaxation of the reaction mode, have been considered (for weak coupling) within Redfield theory. 31 In a recent model study, we have investigated in detail the influence of multidimensional coherent and dissipative vibrational motion on the electron-injection dynamics, 37 employing the self-consistent hybrid approach 38,39 in combination with the multilayer multiconfiguration time- dependent Hartree method. 40 These methods allow an accurate quantum dynamical description of the ET process beyond the limitations of perturbation theory. To apply such models to experimentally studied systems, various model parameters such as the energies and couplings of the relevant electronic states, the important vibrational modes of the chromophore, and the electronic-vibrational couplings need to be determined. If only a single (or a few) reaction mode(s) is considered and a simple model for the donor- acceptor coupling (e.g., the wide-band approximation) is used, then it is possible to determine the parameters empirically based * Authors to whom correspondence should be addressed. E-mail: [email protected] (H.W.) and [email protected] (M.T.). ² Technical University of Munich. ‡ Charles University. § New Mexico State University. | Present address: Institute for Scientific Computing, Forschungszentrum Karlsruhe, P.O. Box 3640, 76021 Karlsruhe, Germany. 11970 J. Phys. Chem. C 2007, 111, 11970-11981 10.1021/jp072217m CCC: $37.00 © 2007 American Chemical Society Published on Web 07/21/2007

Embed Size (px)

Recommended